#------------------------------------------------------------------------------
#$Date: 2025-06-03 22:27:10 +0300 (Tue, 03 Jun 2025) $
#$Revision: 299936 $
#$URL: file:///home/coder/svn-repositories/cod/cif/2/02/34/2023467.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2023467
loop_
_publ_author_name
'Yamane, Hisanori'
'Funahashi, Shiro'
'Hirosaki, Naoto'
'Takeda, Takashi'
_publ_section_title
;
 Orthosilicates with glaserite-type crystal structures:
 Na₂BaZr[SiO₄]₂ and
 Na₂BaHf[SiO₄]₂.
;
_journal_coeditor_code           WM5753
_journal_issue                   'Pt 5'
_journal_name_full
'Acta crystallographica. Section E, Crystallographic communications'
_journal_page_first              368
_journal_page_last               371
_journal_paper_doi               10.1107/S2056989025002956
_journal_volume                  81
_journal_year                    2025
_chemical_formula_iupac          'Na2 Ba Hf [Si O4]2'
_chemical_formula_moiety         'Hf O8 Si2, Ba, 2(Na)'
_chemical_formula_sum            'Ba Hf Na2 O8 Si2'
_chemical_formula_weight         545.99
_chemical_name_systematic
;
Disodium barium hafnium bis(orthosilicate)
;
_space_group_crystal_system      trigonal
_space_group_IT_number           147
_space_group_name_Hall           '-P 3'
_space_group_name_H-M_alt        'P -3'
_atom_sites_solution_primary     dual
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   5.3889(2)
_cell_length_b                   5.3889(2)
_cell_length_c                   7.1996(2)
_cell_measurement_reflns_used    7145
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      50.9650
_cell_measurement_theta_min      2.8010
_cell_volume                     181.067(11)
_computing_cell_refinement
;
CrysAlisPro (Rigaku OD, 2023)
;
_computing_data_collection
;
CrysAlisPro (Rigaku OD, 2023)
;
_computing_data_reduction
;
CrysAlisPro (Rigaku OD, 2023)
;
_computing_molecular_graphics
;
VESTA (Momma & Izumi, 2011)
;
_computing_publication_material
;
Olex2 (Dolomanov et al.,  2009),
publCIF (Westrip, 2010)
;
_computing_structure_refinement
;
SHELXL (Sheldrick, 2015b)
;
_computing_structure_solution
;
SHELXT (Sheldrick, 2015a)
;
_diffrn_ambient_temperature      293(2)
_diffrn_detector                 'Hybrid Pixel Array Detector'
_diffrn_detector_area_resol_mean 10.0000
_diffrn_measured_fraction_theta_full 1.000
_diffrn_measured_fraction_theta_max 1.000
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'ROD, Synergy Custom system, HyPix-Arc 150'
_diffrn_measurement_method       'ω scans'
_diffrn_radiation_monochromator  mirror
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0454
_diffrn_reflns_av_unetI/netI     0.0154
_diffrn_reflns_limit_h_max       7
_diffrn_reflns_limit_h_min       -8
_diffrn_reflns_limit_k_max       8
_diffrn_reflns_limit_k_min       -8
_diffrn_reflns_limit_l_max       11
_diffrn_reflns_limit_l_min       -11
_diffrn_reflns_number            8609
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         34.946
_diffrn_reflns_theta_min         2.829
_diffrn_source                   'Rotating-anode X-ray tube'
_exptl_absorpt_coefficient_mu    20.193
_exptl_absorpt_correction_T_max  0.883
_exptl_absorpt_correction_T_min  0.641
_exptl_absorpt_correction_type   gaussian
_exptl_absorpt_process_details
;
(CrysAlisPro; Rigaku OD, 2023)
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    5.007
_exptl_crystal_description       plate
_exptl_crystal_F_000             242
_exptl_crystal_size_max          0.032
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.008
_refine_diff_density_max         0.609
_refine_diff_density_min         -0.603
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.106
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     24
_refine_ls_number_reflns         538
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.106
_refine_ls_R_factor_all          0.0107
_refine_ls_R_factor_gt           0.0103
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[σ²(Fo²)+(0.0035P)²+0.1631P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0234
_refine_ls_wR_factor_ref         0.0235
_reflns_number_gt                532
_reflns_number_total             538
_reflns_threshold_expression     'I > 2σ(I)'
_cod_data_source_file            wm5753.cif
_cod_data_source_block           II
_cod_depositor_comments
'Adding full bibliography for 2023466--2023467.cif.'
_cod_original_cell_volume        181.067(14)
_cod_database_code               2023467
_shelx_space_group_comment
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_shelx_estimated_absorpt_t_min   0.564
_shelx_estimated_absorpt_t_max   0.855
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-y, x-y, z'
'-x+y, -x, z'
'-x, -y, -z'
'y, -x+y, -z'
'x-y, x, -z'
loop_
_atom_site_type_symbol
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Na Na1 0.333333 0.666667 0.7096(2) 0.0148(2) Uani d 1 . .
Ba Ba1 0.000000 0.000000 0.000000 0.01327(5) Uani d 1 . .
Hf Hf1 0.000000 0.000000 0.500000 0.00516(4) Uani d 1 . .
Si Si1 0.333333 0.666667 0.24191(11) 0.00532(12) Uani d 1 . .
O O1 0.1238(3) 0.3468(3) 0.3269(2) 0.0118(4) Uani d 1 . .
O O2 0.333333 0.666667 0.0232(3) 0.0187(5) Uani d 1 . .
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Na Na 0.0362 0.0249 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ba Ba -0.3244 2.2819 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Hf Hf -0.5830 6.1852 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Si Si 0.0817 0.0704 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_exptl_crystal_face_index_h
_exptl_crystal_face_index_k
_exptl_crystal_face_index_l
_exptl_crystal_face_perp_dist
0 0 -1 0.0057
0 0 1 0.0019
0 1 0 0.0116
-3 -5 1 0.0111
1 -5 0 0.0133
5 -3 -1 0.0116
-5 4 1 0.0145
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
_geom_angle_publ_flag
Si1 Na1 Hf1 4_666 1_565 160.53(5) ?
Si1 Na1 Hf1 4_676 1_565 66.522(10) ?
Si1 Na1 Hf1 4_566 1_565 66.522(10) ?
Si1 Na1 Hf1 . 1_565 64.13(2) ?
Si1 Na1 Si1 4_676 4_666 118.773(12) ?
Si1 Na1 Si1 4_676 4_566 118.773(12) ?
Si1 Na1 Si1 4_566 4_666 118.773(12) ?
Si1 Na1 Si1 4_676 . 96.40(3) ?
Si1 Na1 Si1 4_566 . 96.40(3) ?
Si1 Na1 Si1 4_666 . 96.40(3) ?
O1 Na1 Hf1 4_666 1_565 138.33(5) ?
O1 Na1 Hf1 5_566 1_565 36.38(3) ?
O1 Na1 Hf1 6_556 1_565 86.70(3) ?
O1 Na1 Hf1 4_566 1_565 35.92(4) ?
O1 Na1 Hf1 5_556 1_565 137.65(5) ?
O1 Na1 Hf1 6_666 1_565 85.99(4) ?
O1 Na1 Si1 4_566 4_676 92.15(4) ?
O1 Na1 Si1 4_666 4_666 30.94(3) ?
O1 Na1 Si1 4_566 4_666 148.71(4) ?
O1 Na1 Si1 6_666 4_676 31.12(4) ?
O1 Na1 Si1 5_566 . 84.93(4) ?
O1 Na1 Si1 5_556 4_676 148.71(4) ?
O1 Na1 Si1 5_566 4_666 148.92(3) ?
O1 Na1 Si1 5_566 4_676 30.94(3) ?
O1 Na1 Si1 6_666 . 83.83(5) ?
O1 Na1 Si1 6_556 4_676 148.92(3) ?
O1 Na1 Si1 4_666 . 84.93(4) ?
O1 Na1 Si1 4_666 4_676 91.76(3) ?
O1 Na1 Si1 5_556 4_666 31.12(4) ?
O1 Na1 Si1 4_566 4_566 31.12(4) ?
O1 Na1 Si1 6_556 4_666 91.76(3) ?
O1 Na1 Si1 6_666 4_566 148.71(4) ?
O1 Na1 Si1 4_566 . 83.83(5) ?
O1 Na1 Si1 5_556 4_566 92.15(4) ?
O1 Na1 Si1 5_556 . 83.83(5) ?
O1 Na1 Si1 5_566 4_566 91.76(3) ?
O1 Na1 Si1 6_556 . 84.93(4) ?
O1 Na1 Si1 6_556 4_566 30.94(3) ?
O1 Na1 Si1 4_666 4_566 148.92(3) ?
O1 Na1 Si1 6_666 4_666 92.15(4) ?
O1 Na1 O1 5_556 4_666 57.02(7) ?
O1 Na1 O1 4_566 5_566 62.36(7) ?
O1 Na1 O1 6_666 6_556 168.44(9) ?
O1 Na1 O1 5_556 6_556 62.36(7) ?
O1 Na1 O1 5_556 5_566 168.44(9) ?
O1 Na1 O1 5_566 4_666 119.229(13) ?
O1 Na1 O1 6_666 5_556 118.859(19) ?
O1 Na1 O1 6_556 4_666 119.229(13) ?
O1 Na1 O1 6_666 5_566 57.02(7) ?
O1 Na1 O1 4_566 4_666 168.44(9) ?
O1 Na1 O1 4_566 6_556 57.02(7) ?
O1 Na1 O1 6_666 4_666 62.36(7) ?
O1 Na1 O1 4_566 6_666 118.859(19) ?
O1 Na1 O1 4_566 5_556 118.859(19) ?
O1 Na1 O1 5_566 6_556 119.229(13) ?
O2 Na1 Hf1 1_556 1_565 115.87(2) ?
O2 Na1 Si1 1_556 4_666 83.60(3) ?
O2 Na1 Si1 1_556 . 180.0 ?
O2 Na1 Si1 1_556 4_566 83.60(3) ?
O2 Na1 Si1 1_556 4_676 83.60(3) ?
O2 Na1 O1 1_556 6_556 95.07(4) ?
O2 Na1 O1 1_556 5_556 96.17(5) ?
O2 Na1 O1 1_556 5_566 95.07(4) ?
O2 Na1 O1 1_556 6_666 96.17(5) ?
O2 Na1 O1 1_556 4_566 96.17(5) ?
O2 Na1 O1 1_556 4_666 95.07(4) ?
O1 Ba1 O1 3 . 59.36(5) ?
O1 Ba1 O1 4 . 180.0 ?
O1 Ba1 O1 6 2 120.64(5) ?
O1 Ba1 O1 5 2 180.00(8) ?
O1 Ba1 O1 4 2 120.64(5) ?
O1 Ba1 O1 4 5 59.36(5) ?
O1 Ba1 O1 3 2 59.36(5) ?
O1 Ba1 O1 6 5 59.36(5) ?
O1 Ba1 O1 3 5 120.64(5) ?
O1 Ba1 O1 6 . 120.64(5) ?
O1 Ba1 O1 4 6 59.36(5) ?
O1 Ba1 O1 5 . 120.64(5) ?
O1 Ba1 O1 4 3 120.64(5) ?
O1 Ba1 O1 6 3 180.00(10) ?
O1 Ba1 O1 2 . 59.36(5) ?
O1 Ba1 O2 5 4_665 52.61(5) ?
O1 Ba1 O2 . . 52.61(5) ?
O1 Ba1 O2 6 4_665 108.55(5) ?
O1 Ba1 O2 . 4_665 80.96(5) ?
O1 Ba1 O2 5 4 108.55(5) ?
O1 Ba1 O2 6 1_445 71.45(5) ?
O1 Ba1 O2 3 . 99.04(5) ?
O1 Ba1 O2 5 1_445 127.39(5) ?
O1 Ba1 O2 6 4 99.04(5) ?
O1 Ba1 O2 . 1_445 99.04(5) ?
O1 Ba1 O2 . 4 127.39(5) ?
O1 Ba1 O2 . 4_565 71.45(5) ?
O1 Ba1 O2 6 . 80.96(5) ?
O1 Ba1 O2 4 1_545 71.45(5) ?
O1 Ba1 O2 5 . 71.45(5) ?
O1 Ba1 O2 6 1_545 127.39(5) ?
O1 Ba1 O2 4 4 52.61(5) ?
O1 Ba1 O2 3 1_545 52.61(5) ?
O1 Ba1 O2 3 4 80.96(5) ?
O1 Ba1 O2 5 1_545 80.96(5) ?
O1 Ba1 O2 2 4 71.45(5) ?
O1 Ba1 O2 2 1_545 99.04(5) ?
O1 Ba1 O2 4 4_665 99.04(5) ?
O1 Ba1 O2 . 1_545 108.55(5) ?
O1 Ba1 O2 3 4_665 71.45(5) ?
O1 Ba1 O2 4 . 127.39(5) ?
O1 Ba1 O2 2 4_665 127.39(5) ?
O1 Ba1 O2 4 4_565 108.55(5) ?
O1 Ba1 O2 4 1_445 80.96(5) ?
O1 Ba1 O2 6 4_565 52.61(5) ?
O1 Ba1 O2 3 1_445 108.55(5) ?
O1 Ba1 O2 3 4_565 127.39(5) ?
O1 Ba1 O2 2 1_445 52.61(5) ?
O1 Ba1 O2 5 4_565 99.04(5) ?
O1 Ba1 O2 2 4_565 80.96(5) ?
O1 Ba1 O2 2 . 108.55(5) ?
O2 Ba1 O2 4_565 4_665 119.716(8) ?
O2 Ba1 O2 4_565 4 119.716(8) ?
O2 Ba1 O2 4 1_445 60.285(8) ?
O2 Ba1 O2 1_545 4_665 60.284(8) ?
O2 Ba1 O2 1_545 1_445 119.716(8) ?
O2 Ba1 O2 . 4_665 60.285(8) ?
O2 Ba1 O2 4_565 1_545 180.0 ?
O2 Ba1 O2 4 4_665 119.715(8) ?
O2 Ba1 O2 4_565 1_445 60.284(8) ?
O2 Ba1 O2 . 4 180.0 ?
O2 Ba1 O2 . 1_445 119.715(8) ?
O2 Ba1 O2 4_565 . 60.285(8) ?
O2 Ba1 O2 1_545 4 60.284(8) ?
O2 Ba1 O2 1_545 . 119.715(8) ?
O2 Ba1 O2 4_665 1_445 180.0 ?
Na1 Hf1 Na1 4_566 4_666 102.38(3) ?
Na1 Hf1 Na1 4_566 4_556 102.38(3) ?
Na1 Hf1 Na1 . 1_445 102.38(3) ?
Na1 Hf1 Na1 1_445 4_666 180.0 ?
Na1 Hf1 Na1 1_545 1_445 102.38(3) ?
Na1 Hf1 Na1 1_545 4_566 180.0 ?
Na1 Hf1 Na1 1_545 4_556 77.62(3) ?
Na1 Hf1 Na1 1_545 4_666 77.62(3) ?
Na1 Hf1 Na1 . 4_556 180.0 ?
Na1 Hf1 Na1 . 4_666 77.62(3) ?
Na1 Hf1 Na1 4_566 1_445 77.62(3) ?
Na1 Hf1 Na1 4_556 4_666 102.38(3) ?
Na1 Hf1 Na1 4_556 1_445 77.62(3) ?
Na1 Hf1 Na1 1_545 . 102.38(3) ?
Na1 Hf1 Na1 4_566 . 77.62(3) ?
O1 Hf1 Na1 6_556 1_545 116.29(5) ?
O1 Hf1 Na1 2 1_445 63.71(5) ?
O1 Hf1 Na1 5_556 . 44.07(4) ?
O1 Hf1 Na1 3 1_545 63.71(5) ?
O1 Hf1 Na1 4_556 1_445 58.91(4) ?
O1 Hf1 Na1 4_556 1_545 44.07(4) ?
O1 Hf1 Na1 6_556 4_566 63.71(5) ?
O1 Hf1 Na1 4_556 . 116.29(5) ?
O1 Hf1 Na1 6_556 1_445 44.07(4) ?
O1 Hf1 Na1 5_556 4_566 121.09(4) ?
O1 Hf1 Na1 4_556 4_566 135.93(4) ?
O1 Hf1 Na1 2 4_666 116.29(5) ?
O1 Hf1 Na1 6_556 4_666 135.93(4) ?
O1 Hf1 Na1 . 4_666 58.91(4) ?
O1 Hf1 Na1 5_556 1_445 116.29(5) ?
O1 Hf1 Na1 2 4_556 44.07(4) ?
O1 Hf1 Na1 . 1_445 121.09(4) ?
O1 Hf1 Na1 . 4_556 116.29(5) ?
O1 Hf1 Na1 3 1_445 135.93(4) ?
O1 Hf1 Na1 6_556 4_556 121.09(4) ?
O1 Hf1 Na1 4_556 4_666 121.09(4) ?
O1 Hf1 Na1 3 4_556 58.91(4) ?
O1 Hf1 Na1 . 1_545 135.93(4) ?
O1 Hf1 Na1 4_556 4_556 63.71(5) ?
O1 Hf1 Na1 5_556 4_666 63.71(5) ?
O1 Hf1 Na1 2 4_566 58.91(4) ?
O1 Hf1 Na1 . 4_566 44.07(4) ?
O1 Hf1 Na1 5_556 4_556 135.93(4) ?
O1 Hf1 Na1 3 4_666 44.07(4) ?
O1 Hf1 Na1 2 . 135.93(4) ?
O1 Hf1 Na1 5_556 1_545 58.91(4) ?
O1 Hf1 Na1 . . 63.71(5) ?
O1 Hf1 Na1 2 1_545 121.09(4) ?
O1 Hf1 Na1 6_556 . 58.91(4) ?
O1 Hf1 Na1 3 . 121.09(4) ?
O1 Hf1 Na1 3 4_566 116.29(5) ?
O1 Hf1 O1 5_556 4_556 87.19(7) ?
O1 Hf1 O1 5_556 6_556 87.19(7) ?
O1 Hf1 O1 . 3 87.19(7) ?
O1 Hf1 O1 2 4_556 92.81(7) ?
O1 Hf1 O1 5_556 3 92.81(7) ?
O1 Hf1 O1 . 4_556 180.0 ?
O1 Hf1 O1 2 . 87.19(7) ?
O1 Hf1 O1 6_556 4_556 87.19(7) ?
O1 Hf1 O1 . 6_556 92.81(7) ?
O1 Hf1 O1 3 4_556 92.81(7) ?
O1 Hf1 O1 2 3 87.19(7) ?
O1 Hf1 O1 5_556 2 180.0 ?
O1 Hf1 O1 6_556 3 180.0 ?
O1 Hf1 O1 5_556 . 92.81(7) ?
O1 Hf1 O1 2 6_556 92.81(7) ?
Na1 Si1 Na1 4_676 4_566 118.773(12) ?
Na1 Si1 Na1 4_666 . 83.60(3) ?
Na1 Si1 Na1 4_566 . 83.60(3) ?
Na1 Si1 Na1 4_566 4_666 118.772(12) ?
Na1 Si1 Na1 4_676 . 83.60(3) ?
Na1 Si1 Na1 4_676 4_666 118.772(12) ?
Na1 Si1 Ba1 4_676 1_565 67.724(16) ?
Na1 Si1 Ba1 4_566 1_665 157.16(4) ?
Na1 Si1 Ba1 . . 119.240(11) ?
Na1 Si1 Ba1 4_666 1_565 157.16(4) ?
Na1 Si1 Ba1 . 1_665 119.240(11) ?
Na1 Si1 Ba1 . 1_565 119.240(11) ?
Na1 Si1 Ba1 4_676 1_665 67.723(16) ?
Na1 Si1 Ba1 4_676 . 157.16(4) ?
Na1 Si1 Ba1 4_666 1_665 67.723(16) ?
Na1 Si1 Ba1 4_566 . 67.723(16) ?
Na1 Si1 Ba1 4_666 . 67.723(16) ?
Na1 Si1 Ba1 4_566 1_565 67.724(16) ?
Ba1 Si1 Ba1 . 1_665 98.169(14) ?
Ba1 Si1 Ba1 1_565 . 98.169(14) ?
Ba1 Si1 Ba1 1_565 1_665 98.169(14) ?
O1 Si1 Na1 3_565 4_676 50.52(5) ?
O1 Si1 Na1 2_665 . 68.03(6) ?
O1 Si1 Na1 . 4_676 149.93(7) ?
O1 Si1 Na1 2_665 4_566 149.94(7) ?
O1 Si1 Na1 3_565 4_566 69.22(5) ?
O1 Si1 Na1 3_565 4_666 149.94(7) ?
O1 Si1 Na1 . . 68.03(6) ?
O1 Si1 Na1 . 4_666 69.22(5) ?
O1 Si1 Na1 2_665 4_676 69.22(5) ?
O1 Si1 Na1 2_665 4_666 50.51(5) ?
O1 Si1 Na1 . 4_566 50.51(5) ?
O1 Si1 Na1 3_565 . 68.03(6) ?
O1 Si1 Ba1 . 1_665 134.78(5) ?
O1 Si1 Ba1 3_565 1_565 52.13(6) ?
O1 Si1 Ba1 3_565 1_665 117.23(5) ?
O1 Si1 Ba1 2_665 1_665 52.13(6) ?
O1 Si1 Ba1 . 1_565 117.23(5) ?
O1 Si1 Ba1 2_665 . 117.23(5) ?
O1 Si1 Ba1 . . 52.13(6) ?
O1 Si1 Ba1 2_665 1_565 134.78(5) ?
O1 Si1 Ba1 3_565 . 134.78(6) ?
O1 Si1 O1 3_565 . 106.86(7) ?
O1 Si1 O1 . 2_665 106.86(7) ?
O1 Si1 O1 3_565 2_665 106.86(7) ?
O2 Si1 Na1 . . 180.0 ?
O2 Si1 Na1 . 4_666 96.40(3) ?
O2 Si1 Na1 . 4_566 96.40(3) ?
O2 Si1 Na1 . 4_676 96.40(3) ?
O2 Si1 Ba1 . . 60.760(11) ?
O2 Si1 Ba1 . 1_665 60.760(11) ?
O2 Si1 Ba1 . 1_565 60.760(11) ?
O2 Si1 O1 . . 111.97(6) ?
O2 Si1 O1 . 2_665 111.97(6) ?
O2 Si1 O1 . 3_565 111.97(6) ?
Na1 O1 Na1 4_566 4_666 168.44(9) ?
Na1 O1 Ba1 4_566 . 89.42(6) ?
Ba1 O1 Na1 . 4_666 79.80(5) ?
Hf1 O1 Na1 . 4_666 84.71(5) ?
Hf1 O1 Na1 . 4_566 100.01(6) ?
Hf1 O1 Ba1 . . 92.35(6) ?
Si1 O1 Na1 . 4_566 98.37(7) ?
Si1 O1 Na1 . 4_666 79.84(6) ?
Si1 O1 Ba1 . . 101.12(7) ?
Si1 O1 Hf1 . . 157.27(10) ?
Na1 O2 Ba1 1_554 1_665 86.93(4) ?
Na1 O2 Ba1 1_554 1_565 86.93(4) ?
Na1 O2 Ba1 1_554 . 86.93(4) ?
Ba1 O2 Ba1 1_565 1_665 119.715(8) ?
Ba1 O2 Ba1 . 1_665 119.715(8) ?
Ba1 O2 Ba1 1_565 . 119.715(8) ?
Si1 O2 Na1 . 1_554 180.0 ?
Si1 O2 Ba1 . . 93.07(4) ?
Si1 O2 Ba1 . 1_565 93.07(4) ?
Si1 O2 Ba1 . 1_665 93.07(4) ?
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
_geom_bond_publ_flag
Na1 Hf1 1_565 3.4579(6) ?
Na1 Si1 . 3.3670(16) ?
Na1 Si1 4_676 3.1308(2) ?
Na1 Si1 4_666 3.1308(2) ?
Na1 Si1 4_566 3.1308(2) ?
Na1 O1 5_556 2.4423(15) yes
Na1 O1 4_566 2.4423(15) ?
Na1 O1 6_666 2.4423(15) ?
Na1 O1 6_556 2.9738(15) yes
Na1 O1 5_566 2.9738(15) ?
Na1 O1 4_666 2.9738(15) ?
Na1 O1 . 3.145(2) yes
Na1 O1 3_565 3.145(2) ?
Na1 O1 2_665 3.145(2) ?
Na1 O2 1_556 2.258(3) yes
Ba1 O1 5 2.8687(16) ?
Ba1 O1 3 2.8687(16) ?
Ba1 O1 4 2.8687(16) ?
Ba1 O1 . 2.8687(16) yes
Ba1 O1 6 2.8687(16) ?
Ba1 O1 2 2.8687(16) ?
Ba1 O2 4_565 3.11574(17) ?
Ba1 O2 4_665 3.11577(17) ?
Ba1 O2 4 3.11577(17) ?
Ba1 O2 1_545 3.11574(17) ?
Ba1 O2 . 3.11576(17) yes
Ba1 O2 1_445 3.11577(17) ?
Hf1 O1 5_556 2.0600(15) ?
Hf1 O1 4_556 2.0600(15) ?
Hf1 O1 3 2.0600(15) ?
Hf1 O1 . 2.0600(15) yes
Hf1 O1 6_556 2.0600(15) ?
Hf1 O1 2 2.0600(15) ?
Si1 O1 2_665 1.6354(16) ?
Si1 O1 . 1.6354(16) yes
Si1 O1 3_565 1.6354(16) ?
Si1 O2 . 1.575(2) yes
loop_
_geom_torsion_atom_site_label_1
_geom_torsion_atom_site_label_2
_geom_torsion_atom_site_label_3
_geom_torsion_atom_site_label_4
_geom_torsion_site_symmetry_1
_geom_torsion_site_symmetry_2
_geom_torsion_site_symmetry_3
_geom_torsion_site_symmetry_4
_geom_torsion
_geom_torsion_publ_flag
Na1 Si1 O1 Na1 4_676 . . 4_566 79.72(11) ?
Na1 Si1 O1 Na1 . . . 4_666 -91.40(4) ?
Na1 Si1 O1 Na1 4_566 . . 4_666 168.43(9) ?
Na1 Si1 O1 Na1 4_666 . . 4_566 -168.43(9) ?
Na1 Si1 O1 Na1 4_676 . . 4_666 -111.84(10) ?
Na1 Si1 O1 Na1 . . . 4_566 100.17(6) ?
Na1 Si1 O1 Ba1 4_676 . . . 170.78(6) ?
Na1 Si1 O1 Ba1 . . . . -168.78(6) ?
Na1 Si1 O1 Ba1 4_666 . . . -77.38(5) ?
Na1 Si1 O1 Ba1 4_566 . . . 91.06(7) ?
Na1 Si1 O1 Hf1 4_566 . . . -143.7(3) ?
Na1 Si1 O1 Hf1 4_666 . . . 47.9(2) ?
Na1 Si1 O1 Hf1 4_676 . . . -63.9(3) ?
Na1 Si1 O1 Hf1 . . . . -43.5(2) ?
Na1 Si1 O2 Ba1 4_676 . . 1_565 -60.000000 ?
Na1 Si1 O2 Ba1 4_566 . . . -60.0 ?
Na1 Si1 O2 Ba1 4_676 . . 1_665 60.0 ?
Na1 Si1 O2 Ba1 4_666 . . 1_665 -60.0 ?
Na1 Si1 O2 Ba1 4_666 . . . 60.0 ?
Na1 Si1 O2 Ba1 4_666 . . 1_565 180.0 ?
Na1 Si1 O2 Ba1 4_566 . . 1_665 180.000000 ?
Na1 Si1 O2 Ba1 4_676 . . . 180.0 ?
Na1 Si1 O2 Ba1 4_566 . . 1_565 60.0 ?
Ba1 Si1 O1 Na1 . . . 4_566 -91.06(7) ?
Ba1 Si1 O1 Na1 . . . 4_666 77.38(5) ?
Ba1 Si1 O1 Na1 1_565 . . 4_666 155.97(4) ?
Ba1 Si1 O1 Na1 1_665 . . 4_566 -149.85(6) ?
Ba1 Si1 O1 Na1 1_565 . . 4_566 -12.46(9) ?
Ba1 Si1 O1 Na1 1_665 . . 4_666 18.58(9) ?
Ba1 Si1 O1 Ba1 1_565 . . . 78.60(6) ?
Ba1 Si1 O1 Ba1 1_665 . . . -58.80(9) ?
Ba1 Si1 O1 Hf1 1_565 . . . -156.1(2) ?
Ba1 Si1 O1 Hf1 . . . . 125.3(3) ?
Ba1 Si1 O1 Hf1 1_665 . . . 66.5(3) ?
Ba1 Si1 O2 Ba1 1_665 . . 1_565 -120.0 ?
Ba1 Si1 O2 Ba1 1_665 . . . 120.0 ?
Ba1 Si1 O2 Ba1 1_565 . . . -120.000000 ?
Ba1 Si1 O2 Ba1 . . . 1_565 120.0 ?
Ba1 Si1 O2 Ba1 . . . 1_665 -120.0 ?
Ba1 Si1 O2 Ba1 1_565 . . 1_665 120.0 ?
O1 Si1 O1 Na1 3_565 . . 4_666 -148.46(7) ?
O1 Si1 O1 Na1 3_565 . . 4_566 43.11(12) ?
O1 Si1 O1 Na1 2_665 . . 4_566 157.23(5) ?
O1 Si1 O1 Na1 2_665 . . 4_666 -34.34(9) ?
O1 Si1 O1 Ba1 3_565 . . . 134.17(9) ?
O1 Si1 O1 Ba1 2_665 . . . -111.72(10) ?
O1 Si1 O1 Hf1 3_565 . . . -100.56(19) ?
O1 Si1 O1 Hf1 2_665 . . . 13.6(3) ?
O1 Si1 O2 Ba1 3_565 . . 1_565 -10.14(6) ?
O1 Si1 O2 Ba1 2_665 . . 1_565 -130.14(6) ?
O1 Si1 O2 Ba1 3_565 . . . -130.14(6) ?
O1 Si1 O2 Ba1 . . . . -10.14(6) ?
O1 Si1 O2 Ba1 2_665 . . . 109.86(6) ?
O1 Si1 O2 Ba1 . . . 1_665 -130.14(6) ?
O1 Si1 O2 Ba1 2_665 . . 1_665 -10.14(6) ?
O1 Si1 O2 Ba1 3_565 . . 1_665 109.86(6) ?
O1 Si1 O2 Ba1 . . . 1_565 109.86(6) ?
O2 Si1 O1 Na1 . . . 4_566 -79.83(6) ?
O2 Si1 O1 Na1 . . . 4_666 88.60(4) ?
O2 Si1 O1 Ba1 . . . . 11.22(6) ?
O2 Si1 O1 Hf1 . . . . 136.5(2) ?
